Enhanced Redox Cycle of Rod-Shaped MIL-88A/SnFe2O4@MXene Sheets for Fenton-like Degradation of Congo Red: Optimization and Mechanism

This study intended to fabricate a novel Fenton-like catalyst by supporting the rod-like MIL-88A and the magnetic tin ferrite nanoparticles (SnFe2O4) on the MXene sheets (MIL-88A/SnFe2O4@MXene). The well fabrication and determination of the MIL-88A/SnFe2O4@MXene properties were investigated using SEM, XPS, VSM, Zeta potential, XRD, and FTIR tools. The Fenton-like degradation reaction of CR by MIL-88A/SnFe2O4@MXene was thoroughly studied to identify the optimal proportions of the catalyst components, the impact of CR and H2O2 concentrations, as well as the effect of raising the temperature and the pH medium of the catalytic system and the catalyst dosage. Kinetics studies were executed to analyze the decomposition of CR and H2O2 using First-order and Second-order models. Furthermore, the degradation mechanism was proposed based on the scavenging test that proceeded in the presence of chloroform and t-butanol, in addition to the XPS analysis that clarified the participation of the containing metal species: Fe, Sn, and Ti, and the formation of a continual redox cycle. The obtained intermediates during the CR degradation were defined by GC–MS. A recyclability test was performed on MIL-88A/SnFe2O4@MXene during five runs of the Fenton-like degradation of CR molecules. Finally, the novel MIL-88A/SnFe2O4@MXene Fenton-like catalyst could be recommended as a propitious heterogeneous catalyst with a continuous redox cycle and a recyclability merit.


Introduction
Recently, the world has dug deep into water pollution, threatening the subsistence of freshwater.Undeniably, the excessive utilization of chemicals in varied industries leads to aggravating the water pollution affair.Since draining wastewater from industrial sectors contains many detrimental substances like dissolved metals, phenols, dyes, and polycyclic compounds, the vast jeopardy threatens the presence of adequate freshwater on the earth [1].Particularly, synthetic dyes have innumerable applications, including plastic, leather, hair coloring, paper, textiles, cosmetics, and printing [2].Hence, seventy thousand tons of about one hundred thousand types of dyes are produced annually, and the released percentage of dyes in water bodies ranges from 12 to 15% [3].Unfortunately, these dyes are nondegradable and photostable, so they remain in the aquatic media for a prolonged duration.
Congo red (CR) is an azo dye, applied immensely in textile industries because of its high affinity to cellulose fibers [4].Additionally, CR is used for amyloidosis diagnosing and as a pH indicator.Despite that, CR metabolizes to the carcinogenic benzidine and results in human diseases, such as respiratory and eye diseases, gastrointestinal irritation, and allergies [5].The chemical structure complexity of CR endows it with superhigh stability in aquatic media and high degradation resistance [6].Consequently, purification strategies have been instigated and progressed to conquer the hazard of CR, including precipitation, flocculation, biodegradation, adsorption, ozonation, and advanced oxidation processes (AOPs) [7][8][9][10].
The Fenton process is deemed to be one of the most creditable AOPs that exhibited auspicious application potential in degrading many detrimental contaminants.The Fenton process is distinguished by its excellent efficacy, acceptable cost, low toxicity, and simple operational features [11].There are two types of Fenton reactions: the classical Homo-Fenton reaction proceeded by iron solution and hydrogen peroxide (H 2 O 2 ) to form hydroxyl radicals (•OH), following the Weiss-Haber equation [5].However, Homo-Fenton consumes large concentrations of iron species.Additionally, the degradation aptitude of the Homo-Fenton reaction is controlled by the pH medium of the catalytic system, clarifying a higher performance at a low acidic medium (pH < 3).Hence, it is essential to neutralize the purified water before throwing it out, which renders Homo-Fenton quite costly and monotonous [12].The Hetero-Fenton reaction takes place in a solid/liquid interface since iron or any transition metal species are used in a solid phase, facilitating the catalyst separation and recyclability.Furthermore, the Hetero-Fenton reaction could proceed in a wide pH scale, which is one more merit over the Homo-Fenton reaction [13].Consequently, countless substances have been developed to be efficient Hetero-Fenton catalysts, comprising metal-organic frameworks (MOFs), nanoparticles (NPs), carbon materials, MXene, clays, etc.
The unique characteristics of MOFs, including porous structure, tunable topology, high surface area, mechanical, thermal, and chemical stability, and containing transition metals endow them privilege as Hetero-Fenton catalysts [14,15].Iron-based MOFs like MIL-88A revealed promising potential in Fenton degradation reactions owing to the nontoxicity and accessibility of iron species and the abundantly distributed metal nodes (Fe-O clusters) [16].Nevertheless, the catalytic efficacy of neat iron-based MOFs requires further investigations, where they merely comprise ferric species with weak Fenton activity [17].
MXene is a newborn in the 2D-material family and has lately become a spotlight due to its individual features, comprising hydrophilicity, large surface area, chemical tunability, and good flexibility [18].Hence, MXene has shown superior performance in the wastewater remediation sector, even by adsorption or catalysis [19].Importantly, MXene is a biocompatible substance; therefore, it would not result in a secondary pollutant after the purification process [20].MXene is prepared mainly by HF-etching of MAX; M symbols containing transition metal (Ti, Nb, and V), A represents group element (Sn, Al, and Si), and X could be carbon or nitrogen [21].Nonetheless, the utilization of MXene as a Hetero-Fenton catalyst is still limited, and the catalytic mechanism is not perspicuous.
Tin ferrite (SnFe 2 O 4 ) is one of the bright magnetic nanoparticles that possess propitious merits, such as its ferromagnetic nature, excellent mechanical and chemical stability, and good catalytic activity [22].These merits make SnFe 2 O 4 NPs an eminent Hetero-Fenton catalyst due to the collaboration between Sn and Fe to activate H 2 O 2 and generate •OH radicals [23].Furthermore, the excellent magnetic character provides a perfect catalyst separation after the degradation reaction by a magnet without the conventional separation ways that consume a longer time [24].
Accordingly, we intended to exploit the promising application prospects of MIL-88A, MXene, and SnFe 2 O 4 in wastewater purification to fabricate the novel MIL-88A/SnFe 2 O 4 @ MXene Hetero-Fenton catalyst.Characterization study of the morphological, chemical, structural, and physical characteristics of the MIL-88A/SnFe 2 O 4 @MXene composite was performed by XPS, SEM, XRD, FTIR, VSM, and Zeta potential.A series of Fenton-like degradation experiments of CR by the MIL-88A/SnFe 2 O 4 @MXene/H 2 O 2 system proceeded to determine the optimal degradation conditions.Furthermore, the quenching test was carried out to indicate whether the degradation pathway is radical or nonradical.The degradation mechanism was presumed based on XPS analysis.In addition, the degradation pathway The MIL-88A/SnFe 2 O 4 @MXene catalyst was fabricated using the simple post-synthetic approach, as represented in Scheme 1. MIL-88A and SnFe 2 O 4 NPs were dispersed in 20 mL of distilled water under sonication for 30 min.Then, MXene was mixed with the homogeneous suspension of MIL-88A/SnFe 2 O 4 with continuous sonication for another 30 min.Finally, MIL-88A/SnFe 2 O 4 @MXene was collected and dried at 50 • C for 5 h.MIL-88A/SnFe 2 O 4 @MXene catalysts were prepared by different MIL-88A:MXene ratios: 1:3, 1:1, and 3:1.

Fenton-like Experiments
The optimization of the CR Fenton-like degradation process in the MIL-88A/SnFe 2 O 4 @ MXene/H 2 O 2 system was scrutinized as follows.(1) A comparison test was performed between MIL-88A, SnFe 2 O 4 , MXene, and MIL-88A/SnFe 2 O 4 @MXene to indicate the synergetic effect between the catalytic activities of MIL-88A, SnFe 2 O 4 , and MXene.(2) The pH impact on the catalytic degradation of CR was assessed in a pH range of 3-11.(3) The catalyst dose effect in the efficacy of the catalytic degradation reaction of CR molecules was studied at a dose ranging from 5 to 20 mg.(4) The system temperature influence on the CR degradation% was investigated by verifying the system temperature at the range of 20-50 • C. (5) The oxidant impact on the degradation aptitude of CR molecules was inspected at H 2 O 2 ranging from 10 to 200 mg/L.The CR concentration was increased from 50 to 200 mg/L to define the catalytic activity of MIL-88A/SnFe 2 O 4 @MXene in low and high concentrations of CR molecules.The undegraded concentration of CR was de-tected by spectrophotometer at Lmax = 500 nm, and the degradation% was calculated from Equation (1).
C o is the initial CR concentration, and C t is the undegraded concentration of CR after the Fenton-like degradation process.Scheme 1.The fabrication procedure of the MIL-88A/SnFe2O4@MXene catalyst.

Fenton-like Experiments
The optimization of the CR Fenton-like degradation process in the MIL-88A/SnFe2O4@MXene/H2O2 system was scrutinized as follows.(1) A comparison test was performed between MIL-88A, SnFe2O4, MXene, and MIL-88A/SnFe2O4@MXene to indicate the synergetic effect between the catalytic activities of MIL-88A, SnFe2O4, and MXene.(2) The pH impact on the catalytic degradation of CR was assessed in a pH range of 3-11.(3) The catalyst dose effect in the efficacy of the catalytic degradation reaction of CR molecules was studied at a dose ranging from 5 to 20 mg.(4) The system temperature influence on the CR degradation% was investigated by verifying the system temperature at the range of 20-50 °C.(5) The oxidant impact on the degradation aptitude of CR molecules was inspected at H2O2 ranging from 10 to 200 mg/L.The CR concentration was increased from 50 to 200 mg/L to define the catalytic activity of MIL-88A/SnFe2O4@MXene in low and high concentrations of CR molecules.The undegraded concentration of CR was detected by spectrophotometer at ʎmax = 500 nm, and the degradation% was calculated from Equation (1).
Co is the initial CR concentration, and Ct is the undegraded concentration of CR after the Fenton-like degradation process.

Cycling Test
A cycling test was performed on the magnetic MIL-88A/SnFe2O4@MXene catalyst for five catalytic runs.After completing the catalytic run, the MIL-88A/SnFe2O4@MXene catalyst was collected and washed with acetone to remove the residual CR molecules and the degradation products.After drying the catalyst at 50 °C for 6 h, the regenerated catalyst was used in the next catalytic degradation cycle of CR molecules.

Cycling Test
A cycling test was performed on the magnetic MIL-88A/SnFe 2 O 4 @MXene catalyst for five catalytic runs.After completing the catalytic run, the MIL-88A/SnFe 2 O 4 @MXene catalyst was collected and washed with acetone to remove the residual CR molecules and the degradation products.After drying the catalyst at 50 • C for 6 h, the regenerated catalyst was used in the next catalytic degradation cycle of CR molecules.

Results and Discussions
The active functional groups on the MIL-88A/SnFe 2 O 4 @MXene surface were investigated by the FTIR spectra (Figure 1a).The absorption bands of MIL-88A that were observed at 1605 and 1395 cm −1 are allocated to the asymmetric and symmetric COOH vibrational, sequentially.The belonging absorption band of the Fe-O bond appeared at 571 cm −1 , which confirms the bond formation between the iron species and FA.The absorption bands at 1705 cm −1 are assigned to the C=O group; in addition, the related band to the O-H group manifested at 3375 cm −1 .The carbon-containing groups of MIL-88A appeared at 982 cm −1 (C-H) and 1716 cm −1 (C-C).The spectrum of SnFe 2 O 4 clarified its characteristic peaks at wavenumbers of 707 and 580 cm −1 , which corresponded to Sn-O and Fe-O, respectively.The absorption band at 1630 cm −1 corresponds to O-H bending vibrational, and the broadband at 3395 cm −1 relates to O-H stretching.The spectrum of MXene illustrated the belonging absorption peaks of Ti-C, C-F, and Ti-O at the wavenumbers of 523, 1249, and 630 cm −1 , respectively.The accompanying bands of O-H bending appeared at 1456 cm −1 , and O-H stretching manifested at 3647 cm −1 .The distinctive absorption bands of MIL-88A, SnFe 2 O 4 , and MXene were observed in the spectrum of MIL-88A/SnFe 2 O 4 @MXene, ensuring their binding to form the composite., corresponded to the planes of 002, 006, 008, 0010, 0012, and 110, sequentially [28].The pattern of MIL-88A/SnFe 2 O 4 @MXene confirmed the binding of MIL-88A, SnFe 2 O 4 , and MXene, where the distinguishing peaks of them were observed in the composite pattern.

VSM
The magnetism hysteresis loops of SnFe 2 O 4 and MIL-88A/SnFe 2 O 4 @MXene are represented in Figure 1c.The coercivity magnitudes of SnFe 2 O 4 and MIL-88A/SnFe 2 O 4 @MXene were 188.96 and 176.95 G, reflecting their soft ferromagnetic character.Moreover, the saturation magnetization values of SnFe 2 O 4 and MIL-88A/SnFe 2 O 4 @MXene were 43.95 and 14.19 emu/g, respectively, clarifying a decline in the magnetic property of MIL-88A/SnFe 2 O 4 @MXene compared to SnFe 2 O 4 .This observation owes to the nonmagnetic properties of MIL-88A and MXene.Despite the lower magnetism of MIL-88A/SnFe 2 O 4 @ MXene than the authentic SnFe 2 O 4 , the magnetism of the composite enables it to be an easily separable catalyst.

Zeta Potential
The carried charges on the surface of the MIL-88A/SnFe 2 O 4 @MXene composite were detected using zeta potential analysis, as represented in Figure 1d.The zeta potential results depicted that MIL-88A/SnFe 2 O 4 @MXene carried zero charge when pH = 5.58.This finding implied that MIL-88A/SnFe 2 O 4 @MXene carried positive charges when the pH medium was lower than 5.58 and attained the maximal positive charges (22.21 mV) at pH = 3.When pH was elevated over 5.58, the net charges on the composite's surface were negative, reaching −30.60 mV at pH = 11.
The tin spectrum (Figure 3d) revealed the characteristic peaks of Sn II and Sn IV at 486.37 and 494.64 eV, sequentially [33].The carbon spectrum (Figure 3e

The Impact of the Catalytic pH Medium
The pH of the catalytic medium significantly impacts the Fenton-like degradation aptitude of CR dye; therefore, the degradation process was scrutinized in a wide pH scale (3)(4)(5)(6)(7)(8)(9)(10)(11) for 30 min, as demonstrated in Figure 4b.It was deduced that a highly acidic medium is the best pH medium to degrade CR since its degradation% was 94.54% after 30 min at pH = 3. Whereas, when pH is augmented to near alkaline media, hydroxy iron may precipitate, as elucidated in Equation ( 2), declining the concentration of the iron species in the catalytic medium.Furthermore, when pH increased to alkaline media, the Fentonlike degradation of CR dwindled, which is most likely due to the interaction between the abundant hydroxyl ions with H2O2 to form hydroperoxy anions (Equations ( 3) and ( 4)), which possess a superior affinity to metal species.This is in addition to the possible autodecomposition of hydrogen peroxide to carbon dioxide and water at high alkaline media (Equation ( 5)), which decreases the produced amounts of •OH radicals.

The Impact of the Catalytic pH Medium
The pH of the catalytic medium significantly impacts the Fenton-like degradation aptitude of CR dye; therefore, the degradation process was scrutinized in a wide pH scale (3)(4)(5)(6)(7)(8)(9)(10)(11) for 30 min, as demonstrated in Figure 4b.It was deduced that a highly acidic medium is the best pH medium to degrade CR since its degradation% was 94.54% after 30 min at pH = 3. Whereas, when pH is augmented to near alkaline media, hydroxy iron may precipitate, as elucidated in Equation ( 2), declining the concentration of the iron species in the catalytic medium.Furthermore, when pH increased to alkaline media, the Fenton-like degradation of CR dwindled, which is most likely due to the interaction between the abundant hydroxyl ions with H 2 O 2 to form hydroperoxy anions (Equations ( 3) and ( 4)), which possess a superior affinity to metal species.This is in addition to the possible autodecomposition of hydrogen peroxide to carbon dioxide and water at high alkaline media (Equation ( 5)), which decreases the produced amounts of •OH radicals.
Indeed, H 2 O 2 is the dynamic force of the Fenton/Fenton-like reactions, so the influence of increasing the H 2 O 2 concentrations on the degradation% of CR dye was studied, as shown in Figure 4c.An amelioration was observed in the degradation% of CR molecules from 71.25 to 94.54% after 30 min when the concentration of H 2 O 2 elevated from 10 to 100 mg/L, which could be explained by fostering the production of •OH radicals with the augmentation of the oxidant concentrations.Nevertheless, over-raising in the H 2 O 2 concentrations beyond 100 mg/L worsened the Fenton-like degradation aptitude of CR, which could be due to the possibility of interacting the excess concentrations of H 2 O 2 with the presented •OH to form hydroperoxy radicals (Equation ( 6)).This hydroperoxy could attack the distributed •OH in the catalytic medium and degrade to water and oxygen, as elucidated in Equation ( 7).
3.2.4.The Impact of MIL-88A/SnFe 2 O 4 @MXene Dose Figure 5a reveals the impact of the catalyst dosage study on the efficacy of the Fenton-like degradation reaction of CR dye.A noticeable improvement in the degra-dation% of CR from 79.90 to 99.35% was recorded after 30 min when raising the MIL-88A/SnFe 2 O 4 @MXene dose.This catalytic activity enhancement with elevating the catalyst dose is attributed to boosting the generation of the •OH concentration, which directly reinforced the degradation of CR molecules.

The Impact of the Temperature of the Catalytic System
The influence of the temperature of the catalytic system on the degradation of CR dye by MIL-88A/SnFe 2 O 4 @MXene catalyst was scrutinized at a temperature range of 20-50 • C (Figure 5b) at pH 3 and 30 min of reaction time.The Fenton-like degradation of CR increased until almost 100% when the temperature of the catalytic system elevated to 50 • C.This performance could be ascribed to boosting the interaction between MIL-88A/SnFe 2 O 4 @MXene and H 2 O 2 at higher temperatures, giving rise to fostering the production of the •OH radicals [34].

The Impact of the Concentration of CR Molecules
The degradation activity of MIL-88A/SnFe 2 O 4 @MXene towards different CR concentrations was studied within 1 h (Figure 5c).A synergistic effect was noticed between adsorption and Fenton-like degradation processes; the first step involved the adsorption of CR dye onto the surface of the MIL-88A/SnFe 2 O 4 @MXene catalyst in which the ad-sorption% values of CR were 47.25, 35.73, 25.54, and 18.90% after 10 min when the CR concentrations were 50, 100, 200, and 300 mg/L, respectively.Then, the second step began after adding H 2 O 2 , revealing that the Fenton-like degradation% of CR dye attained 98.31, 84.94, 76.43, and 61.37% at CR concentrations of 50, 100, 200, and 300 mg/L, respectively, after 60 min.

Kinetic Study of H 2 O 2 Decomposition
The decomposition of H 2 O 2 by MIL-88A/SnFe 2 O 4 @MXene catalyst controls the concentration of the generated •OH radicals and directly the efficacy of the degradation of CR molecules.Consequently, the kinetics of the H 2 O 2 decomposition by MIL-88A/SnFe 2 O 4 @MXene was scrutinized, in the absence of CR dye (Figure 5d).The decomposition percent of H 2 O 2 with a concentration of 100 mg/L reached 97.04% after 60 min.
Figure 5a reveals the impact of the catalyst dosage study on the efficacy of the Fentonlike degradation reaction of CR dye.A noticeable improvement in the degradation% of CR from 79.90 to 99.35% was recorded after 30 min when raising the MIL-88A/SnFe2O4@MXene dose.This catalytic activity enhancement with elevating the catalyst dose is attributed to boosting the generation of the •OH concentration, which directly reinforced the degradation of CR molecules.

CR Decomposition
The experimental results from the Fenton-like degradation of CR in the catalytic MIL-88A/SnFe 2 O 4 @MXene/H 2 O 2 system were analyzed using First-order and Second-order models (Equations ( 8) and ( 9)).
C t and C o are the concentrations of CR dye at a time t and initial reaction time, respectively.k 1 and k 2 are the First-order and Second-order rate constants, sequentially.
The kinetic analysis (Figure 6a,b) implied that obeying the Fenton-like degradation of CR by MIL-88A/SnFe 2 O 4 @MXene catalyst to the Second-order model owes to the higher R 2 values that are derived from the Second-order model (Table 1) [35].Moreover, the Fenton-like rate constants at the CR concentrations of 50, 100, 200, and 300 mg/L were 0.4098, 0.0615, 0.0322, and 0.0166 min −1 , respectively, reflecting the high reaction rate constant, at low CR concentration.

H2O2 Decomposition
The decomposition of H2O2 by MIL-88A/SnFe2O4@MXene catalyst was inspected by First-order and Second-order models.Figure 6c,d imply that the decomposition of H2O2 obeyed the First-order model, in which the obtained R 2 values from First-order and Second-order plots were 0.965 and 0.904, respectively.Furthermore, the rate constant of H2O2, based on the First-order model, was 0.0555 min −1 .

Scavenging Test
Figure 7a illustrates the scavenging test of the Fenton-like degradation reaction of CR by MIL-88A/SnFe2O4@MXene catalyst.Generally, chloroform (CF) quenches O2• − radicals, and t-butanol (t-BuOH) hinders •OH radicals [36].The scavenging test revealed a trivial effect of CF on the efficacy of the Fenton-like reaction of CR by the MIL-88A/SnFe2O4@MXene/H2O2 system.On the contrary, t-BuOH dwindled almost half of the activity of MIL-88A/SnFe2O4@MXene towards the degradation of CR molecules.These re-  The decomposition of H 2 O 2 by MIL-88A/SnFe 2 O 4 @MXene catalyst was inspected by First-order and Second-order models.Figure 6c,d imply that the decomposition of H 2 O 2 obeyed the First-order model, in which the obtained R 2 values from First-order and Second-order plots were 0.965 and 0.904, respectively.Furthermore, the rate constant of H 2 O 2 , based on the First-order model, was 0.0555 min −1 .

Scavenging Test
Figure 7a illustrates the scavenging test of the Fenton-like degradation reaction of CR by MIL-88A/SnFe 2 O 4 @MXene catalyst.Generally, chloroform (CF) quenches O 2 • − radicals, and t-butanol (t-BuOH) hinders •OH radicals [36].The scavenging test revealed a trivial effect of CF on the efficacy of the Fenton-like reaction of CR by the MIL-88A/SnFe 2 O 4 @MXene/H 2 O 2 system.On the contrary, t-BuOH dwindled almost half of the activity of MIL-88A/SnFe 2 O 4 @MXene towards the degradation of CR molecules.These results proved that •OH radicals are the controlling reactive groups on the Fenton-like reaction of CR molecules inside the MIL-88A/SnFe 2 O 4 @MXene/H 2 O 2 system.Additionally, the radical pathway is the following pathway of the Fenton-like degradation reaction of CR, not the oxygen vacancies pathway [37].
Nanomaterials 2024, 14, x FOR PEER REVIEW 13 of 19 reaction of CR molecules inside the MIL-88A/SnFe2O4@MXene/H2O2 system.Additionally, the radical pathway is the following pathway of the Fenton-like degradation reaction of CR, not the oxygen vacancies pathway [37].

Degradation Mechanism
In the light of the experimental work, the degradation of CR molecules by MIL-88A/SnFe2O4@MXene composite proceeded by the synergistic effect between adsorption and Fenton-like processes.Firstly, the adsorption of CR molecules onto the active binding sites of MIL-88A/SnFe2O4@MXene was proved from the XPS survey of the used composite (Figure 7b), where the belonging peaks of sulfur-and nitrogen-containing CR appeared at the binding energy of 169.95 and 401.11 eV, respectively.The adsorption process of CR onto MIL-88A/SnFe2O4@MXene was supposed to occur via the coordination bonds between the amine-containing CR molecules and the metal species of MIL-88A/SnFe2O4@MXene: Ti, Sn, and Fe.Furthermore, the potent electrostatic interaction could occur between the cationic active sites of MIL-88A/SnFe2O4@MXene (zeta potential = 22.21 mV at pH = 3) and the anionic CR molecules.Notably, the H-bonding drastically contributed to the adsorption of CR onto MIL-88A/SnFe2O4@MXene since the oxygen and nitrogen atoms of CR molecules and the abundant hydrogen atoms onto the composite surface could attach via H-bonds.In addition, the oxygenated functional groups onto the backbone of MIL-88A/SnFe2O4@MXene could form H-bonds with the hydrogen atoms of the CR molecules.
Secondly, the Fenton-like degradation process of CR molecules proceeded by the activation of H2O2 as follows.

(i)
Fe II species could transfer electrons to activate H2O2 and form •OH radicals, following the Haber-Weiss mechanism, as represented in Equation ( 10).This proposition was proved by the blue shift of the Fe2p spectrum of the used MIL-88A/SnFe2O4@MXene catalyst (Figure 7c).In addition, the Fe III /Fe II ratio of the used catalyst was found to be 0.549, while the ratio of the pure catalyst was 0.264, reflecting the increase in the Fe III amounts after the Fenton-like degradation of CR and contributing of Fe II species in the H2O2 activation.

Degradation Mechanism
In the light of the experimental work, the degradation of CR molecules by MIL-88A/SnFe 2 O 4 @MXene composite proceeded by the synergistic effect between adsorption and Fenton-like processes.Firstly, the adsorption of CR molecules onto the active binding sites of MIL-88A/SnFe 2 O 4 @MXene was proved from the XPS survey of the used composite (Figure 7b), where the belonging peaks of sulfur-and nitrogen-containing CR appeared at the binding energy of 169.95 and 401.11 eV, respectively.The adsorption process of CR onto MIL-88A/SnFe 2 O 4 @MXene was supposed to occur via the coordination bonds between the amine-containing CR molecules and the metal species of MIL-88A/SnFe 2 O 4 @MXene: Ti, Sn, and Fe.Furthermore, the potent electrostatic interaction could occur between the cationic active sites of MIL-88A/SnFe 2 O 4 @MXene (zeta potential = 22.21 mV at pH = 3) and the anionic CR molecules.Notably, the H-bonding drastically contributed to the adsorption of CR onto MIL-88A/SnFe 2 O 4 @MXene since the oxygen and nitrogen atoms of CR molecules and the abundant hydrogen atoms onto the composite surface could attach via H-bonds.In addition, the oxygenated functional groups onto the backbone of MIL-88A/SnFe 2 O 4 @MXene could form H-bonds with the hydrogen atoms of the CR molecules.
Secondly, the Fenton-like degradation process of CR molecules proceeded by the activation of H 2 O 2 as follows.
(i) Fe II species could transfer electrons to activate H 2 O 2 and form •OH radicals, following the Haber-Weiss mechanism, as represented in Equation (10).This proposition was proved by the blue shift of the Fe2p spectrum of the used MIL-88A/SnFe 2 O 4 @MXene catalyst (Figure 7c).In addition, the Fe III /Fe II ratio of the used catalyst was found to be 0.549, while the ratio of the pure catalyst was 0.264, reflecting the increase in the Fe III amounts after the Fenton-like degradation of CR and contributing of Fe II species in the H 2 O 2 activation.
(ii) The Sn II ions play a dual role in the Fenton-like degradation of CR molecules since they could provide the needed electrons to activate H 2 O 2 and produce •OH radicals (Equation ( 11)).The participation of Sn II species in the H 2 O 2 activation was confirmed by the detected shifting in the Sn3d peaks and the increase in the Sn IV /Sn II ratio after the Fenton-like reaction from 0.599 to 0.674 (Figure 7d); additionally, the ability of Sn II to recover Fe III to Fe II , where the redox potential (E o ) of Sn II /Sn IV is 0.14 V, and the E o of Fe II /Fe III is 0.77 V (Equation ( 12)).
Sn II + 2Fe III → 2Fe II + Sn IV (12) (iii) The abundant Ti species (Figure 7e) also contribute to the •OH generation and recover both Fe II and Sn II species.The Ti II and Ti III ions activated H 2 O 2 , as elucidated in Equations ( 13) and ( 14).The lower E o value of Ti II /Ti III compared to Ti III /Ti IV implies a higher affinity of Ti II to activate H 2 O 2 than Ti III .Also, the Ti III /Ti II ratio drastically increased from 1.3 to 16.87, while the ratio of Ti III /Ti IV trivially augmented from 0.274 to 0.277, which reflected the lower contribution of Ti III in the Fenton-like degradation of CR.Such a low E o value of Ti II /Ti III enables it to recover Fe II and Sn II species and sustains the Fenton-like reaction for a long time (Equations ( 15) and ( 16)).These suggestions explained the dramatic decline in the atomic percent of Ti II ions and denoted the significance of MXene in the reducibility of iron and tin [38].Figure 8 exhibits the adsorption and Fenton-like degradation mechanisms of CR by MIL-88A/SnFe 2 O 4 @MXene.

Degradation Pathway of CR Molecules
The degradation pathway of the Fenton-like degradation of CR molecules by MIL-88A/SnFe 2 O 4 @MXene was detected by GC-MS (Figure S1).The decomposition of the CR molecules was supposed to proceed by cleaving of the azo bond, as elucidated in Figure 9, forming benzidine in one pathway at a retention time (RT) of 6.06 min, and 3,4-diaminonaphthalene-1-sulfonic acid in another pathway at RT = 12.67 min.In the first pathway, benzidine converted to 1,1 ′ -biphenyl (RT = 7.5 min) via a deamination reaction, and then it further oxidized to benzene propanoic acid (RT = 24.91 min) and phenol (RT = 6.98 min).In the second pathway, 3,4-diamino naphthalene-1-sulfonic acid converted to naphthalene (RT = 23.27min) via desulfonation and deamination reactions that oxidized to benzene dicarboxylic acid (RT = 27.66 min).

Degradation Pathway of CR Molecules
The degradation pathway of the Fenton-like degradation of CR molecules by MIL-88A/SnFe2O4@MXene was detected by GC-MS (Figure S1).The decomposition of the CR molecules was supposed to proceed by cleaving of the azo bond, as elucidated in Figure 9, forming benzidine in one pathway at a retention time (RT) of 6.06 min, and 3,4-diaminonaphthalene-1-sulfonic acid in another pathway at RT = 12.67 min.In the first pathway, benzidine converted to 1,1′-biphenyl (RT = 7.5 min) via a deamination reaction, and then it further oxidized to benzene propanoic acid (RT = 24.91 min) and phenol (RT = 6.98 min).In the second pathway, 3,4-diamino naphthalene-1-sulfonic acid converted to naphthalene (RT = 23.27min) via desulfonation and deamination reactions that oxidized to benzene dicarboxylic acid (RT = 27.66 min).

Recyclability Test
The recyclability test was performed on MIL-88A/SnFe2O4@MXene after the Fentonlike degradation reaction of CR molecules for five runs, as represented in Figure 10.The experimental result indicated the pre-eminent recyclability of the MIL-88A/SnFe2O4@MXene catalyst, in which its catalytic activity toward the Fenton-like degradation of CR dwindled by 12.61% after the 5th catalytic run.This finding may be as-

Recyclability Test
The recyclability test was performed on MIL-88A/SnFe 2 O 4 @MXene after the Fentonlike degradation reaction of CR molecules for five runs, as represented in Figure 10.The experimental result indicated the pre-eminent recyclability of the MIL-88A/SnFe 2 O 4 @MXene catalyst, in which its catalytic activity toward the Fenton-like degradation of CR dwindled by 12.61% after the 5th catalytic run.This finding may be ascribed to the magnetic property of the catalyst that eases its separation without weight loss.Furthermore, the continuous redox cycle between Fe/Sn/Ti species in the MIL-88A/SnFe 2 O 4 @MXene catalyst increases its activity for a longer time.

Leaching Test
For confirming the durability of the MIL-88A/SnFe2O4@MXene catalyst, the metals leaching from the catalyst were determined by ICP-OES.It was recorded that the leaching concentrations of Fe, Sn, and Ti were 0.01, 0.007, and 0.009 mg/L, respectively.These results indicated the stability of the chemical structure of the MIL-88A/SnFe2O4@MXene catalyst.Furthermore, these low leaching concentrations of the metal-containing MIL-88A/SnFe2O4@MXene reflected the nontoxicity of the catalyst, where it does not result in the formation of secondary pollutants.

Conclusions
The MIL-88A/SnFe2O4@MXene catalyst revealed eminent Fenton-like degradation performance toward CR molecules, where the degradation% almost attained 100% during 60 min.Furthermore, the experimental work exhibited the synergistic effect between adsorption and Fenton-like processes to degrade CR molecules since the adsorption% was 47.25% at 50 mg/L of the CR.The superior Fenton-like degradation of CR was recorded at the catalytic reaction conditions of pH = 3, catalyst dose = 10 mg, CR concentration = 50 mg/L, H2O2 concentration = 100 mg/L, and system temperature = 55 °C.The kinetic study denoted fitting the CR decomposition to the Second-order model and H2O2 decomposition to the First-order model.The scavenger test implied the predominance of •OH radicals on the CR degradation by the MIL-88A/SnFe2O4@MXene/H2O2 catalytic system.The adsorption mechanism of the CR degradation was presumed to proceed by two processes: the adsorption process that occurred via H-bonding, coordination bond, and electrostatic interaction between CR molecules and MIL-88A/SnFe2O4@MXene, in addition to the Fenton-like degradation that is controlled by the formation of the sustainable redox cycle between Sn, Ti, and Fe species.Interestingly, MIL-88A/SnFe2O4@MXene showed an excellent Fenton-like degradation behavior toward the CR molecules during five sequential runs, reflecting the superior recyclability of the catalyst.Nevertheless, the high cost of MXene and MIL-88A limits the study to integration from a lab scale.Consequently, excessive investigations are still needed to find preparation approaches to MXene and MOFs with a lower capital cost.

Supplementary Materials:
The following supporting information can be downloaded at:

Leaching Test
For confirming the durability of the MIL-88A/SnFe 2 O 4 @MXene catalyst, the metals leaching from the catalyst were determined by ICP-OES.It was recorded that the leaching concentrations of Fe, Sn, and Ti were 0.01, 0.007, and 0.009 mg/L, respectively.These results indicated the stability of the chemical structure of the MIL-88A/SnFe 2 O 4 @MXene catalyst.Furthermore, these low leaching concentrations of the metal-containing MIL-88A/SnFe 2 O 4 @MXene reflected the nontoxicity of the catalyst, where it does not result in the formation of secondary pollutants.

Conclusions
The MIL-88A/SnFe 2 O 4 @MXene catalyst revealed eminent Fenton-like degradation performance toward CR molecules, where the degradation% almost attained 100% during 60 min.Furthermore, the experimental work exhibited the synergistic effect between adsorption and Fenton-like processes to degrade CR molecules since the adsorption% was 47.25% at 50 mg/L of the CR.The superior Fenton-like degradation of CR was recorded at the catalytic reaction conditions of pH = 3, catalyst dose = 10 mg, CR concentration = 50 mg/L, H 2 O 2 concentration = 100 mg/L, and system temperature = 55 • C. The kinetic study denoted fitting the CR decomposition to the Second-order model and H 2 O 2 decomposition to the First-order model.The scavenger test implied the predominance of •OH radicals on the CR degradation by the MIL-88A/SnFe 2 O 4 @MXene/H 2 O 2 catalytic system.The adsorption mechanism of the CR degradation was presumed to proceed by two processes: the adsorption process that occurred via H-bonding, coordination bond, and electrostatic interaction between CR molecules and MIL-88A/SnFe 2 O 4 @MXene, in addition to the Fenton-like degradation that is controlled by the formation of the sustainable redox cycle between Sn, Ti, and Fe species.Interestingly, MIL-88A/SnFe 2 O 4 @MXene showed an excellent Fentonlike degradation behavior toward the CR molecules during five sequential runs, reflecting

3395 cm − 1
relates to O-H stretching.The spectrum of MXene illustrated the belonging absorption peaks of Ti-C, C-F, and Ti-O at the wavenumbers of 523, 1249, and 630 cm −1 , respectively.The accompanying bands of O-H bending appeared at 1456 cm −1 , and O-H stretching manifested at 3647 cm −1 .The distinctive absorption bands of MIL-88A, SnFe2O4, and MXene were observed in the spectrum of MIL-88A/SnFe2O4@MXene, ensuring their binding to form the composite.

3. 1
.5.SEM The outer shapes of MIL-88A, SnFe 2 O 4 , MXene, and MIL-88A/SnFe 2 O 4 @MXene were studied using SEM (Figure 2a-d).It was observed that MIL-88A has a rod-like shape, which is the typical shape of the hydrothermally fabricated MIL-88A.The particles of the SnFe 2 O 4 shape are spheroidal, forming high aggregations owing to the high ferromagnetic character of SnFe 2 O 4 , as proven by VSM.The SEM of MXene elucidates exfoliated thin sheets with a rough surface, endowing it a feature to be a good supporter.The SEM of MIL-88A/SnFe 2 O 4 @MXene shows the distribution of the rod-like shape of MIL-88A and the spheroidal SnFe 2 O 4 on the sheets of MXene.Nanomaterials 2024, 14, x FOR PEER REVIEW 7 of 19
) represents the carbonbased functional groups of C-O, O=C-O, and C-C at the binding energies of 285.96, 288.48, and 284.74 eV, respectively.The oxygen spectrum exhibited peaks at 531.85, 529.78, and 531.20 eV, which are assigned to Sn/Fe-O, Ti-O-Ti, and Ti-O-Sn/Fe, sequentially

Figure 9 .
Figure 9. Proposed degradation mechanism of CR molecules based on GC-MS analysis.

Figure 9 .
Figure 9. Proposed degradation mechanism of CR molecules based on GC-MS analysis.

Table 1 .
Derived parameter of the kinetic study of the Fenton-like degradation of CR by MIL-88A/SnFe2O4@MXene catalyst.

Table 1 .
Derived parameter of the kinetic study of the Fenton-like degradation of CR by MIL-88A/SnFe 2 O 4 @MXene catalyst.